High-pressure and low-temperature structural study of claudetite I, a monoclinic layered As2O3 polymorph
Guńka, Piotr A.; Hanfland, Michael; Chen, Yu-Sheng; Zachara, Janusz; CrystEngComm 23 (2021) 638–644; doi:10.1039/D0CE01401J

data_7241831
_publ_section_title
;
 High-pressure and low-temperature structural study of claudetite I, a
 monoclinic layered As2O3 polymorph
;
_journal_issue                   3
_journal_name_full               CrystEngComm
_journal_page_first              638
_journal_page_last               644
_journal_paper_doi               10.1039/D0CE01401J
_journal_volume                  23
_journal_year                    2021
_chemical_formula_moiety         'As2 O3'
_chemical_formula_sum            'As2 O3'
_chemical_formula_weight         197.84
_chemical_name_common            'claudetite I'
_chemical_name_systematic
;
arsenic(III) oxide
;
_space_group_IT_number           14
_space_group_name_Hall           '-P 2yn'
_space_group_name_H-M_alt        'P 1 21/n 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_H-M   'P 1 21/n 1'
_audit_creation_date             2020-10-21T14:02
_audit_creation_method           'created in GSAS-II'
_audit_update_record
;
2020-10-22 deposited with the CCDC.	2020-12-10 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 94.807(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.6166(4)
_cell_length_b                   11.5551(5)
_cell_length_c                   4.05120(28)
_cell_measurement_pressure       2.527e7(5)
_cell_measurement_temperature    293
_cell_volume                     215.35(3)
_computing_data_reduction        Fit2D
_computing_structure_refinement
'GSAS-II (Toby & Von Dreele, J. Appl. Cryst. 46, 544-549, 2013)'
_diffrn_ambient_pressure         2.527e7(5)
_diffrn_ambient_temperature      293
_diffrn_detector                 'Mar555 flat panel'
_diffrn_detector_type            'Mar555 flat panel'
_diffrn_measurement_device_type  'ESRF ID09A beamline'
_diffrn_radiation_monochromator  Si
_diffrn_radiation_polarisn_ratio 0.9900
_diffrn_radiation_probe          x-ray
_diffrn_radiation_wavelength     0.41421
_diffrn_source                   'ESRF ID09A'
_diffrn_source_type              synchrotron
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    6.1020
_exptl_crystal_description       'white powder'
_pd_block_id                     2020-10-21T14:02|clau1_020rietveld||id09a
_pd_calc_method                  'Rietveld Refinement'
_pd_meas_number_of_points        1833
_pd_phase_name                   claudetiteI
_pd_prep_pressure                100.0(1)
_pd_prep_temperature             293
_pd_proc_info_datetime           2020-10-21T14:02
_pd_proc_ls_background_function
;
Background function: "chebyschev" function with 15 terms:
    802.2(16), 272(8), 10(4)e1, 6.4(11)e2, -2.3(4)e3, -4.7(5)e3, 
    1.47(13)e4, 1.39(7)e4, -4.48(15)e4, -1.995(9)e4, 6.74(5)e4, 
    1.38(8)e4, -4.90(19)e4, -3.7(4)e3, 1.39(9)e4, 
;
_pd_proc_ls_pref_orient_corr
;
Simple spherical harmonic correction Order = 6
    Coefficients:  0:0:C(6,6) = -0.008(23); 0:0:C(4,4) = 0.320(21); 
    0:0:C(6,-2) = -0.245(29); 0:0:C(2,-2) = 0.039(16); 0:0:C(4,-4) = -0.222(20); 
    0:0:C(2,2) = 0.416(16); 0:0:C(4,0) = -0.367(19); 0:0:C(6,-6) = -0.146(28); 
    0:0:C(6,4) = -0.171(25); 0:0:C(4,2) = -0.326(20); 0:0:C(6,2) = 0.001(26); 
    0:0:C(6,-4) = 0.111(20); 0:0:C(6,0) = -0.152(24); 0:0:C(2,0) = -0.274(13); 
    0:0:C(4,-2) = -0.095(23); 
;
_pd_proc_ls_profile_function
;
Finger-Cox-Jephcoat function parameters U, V, W, X, Y, SH/L:
  peak variance(Gauss) = Utan(Th)^2^+Vtan(Th)+W:
  peak HW(Lorentz) = X/cos(Th)+Ytan(Th); SH/L = S/L+H/L
  U, V, W in (centideg)^2^, X & Y in centideg
    5.4(4)e3, -8.1(6)e2, 35.2(26), 182.5(9), -27(11), 0.002, 
  Crystallite size in microns with "isotropic" model:
  parameters: Size, G/L mix
    1.000, 1.000, 
  Microstrain, "isotropic" model (10^6^ * delta Q/Q)
    parameters: Mustrain, G/L mix
    1000.000, 1.000, 

;
_pd_proc_ls_prof_R_factor        0.01069
_pd_proc_ls_prof_wR_expected     0.03383
_pd_proc_ls_prof_wR_factor       0.01586
_refine_ls_goodness_of_fit_all   0.477
_refine_ls_matrix_type           full
_refine_ls_number_parameters     57
_refine_ls_R_Fsqd_factor         0.04166
_refine_ls_shift/su_max          0.0008
_refine_ls_wR_factor_obs         0.01588
_reflns_d_resolution_high        1.110
_reflns_d_resolution_low         3.811
_reflns_limit_h_max              4
_reflns_limit_h_min              0
_reflns_limit_k_max              10
_reflns_limit_k_min              0
_reflns_limit_l_max              3
_reflns_limit_l_min              -3
_reflns_number_total             164
_cod_data_source_file            d0ce01401j3.cif
_cod_data_source_block           clau1_020rietveld
_cod_depositor_comments
'Adding full bibliography for 7241824--7241862.cif.'
_cod_original_cell_volume        215.354(11)
_cod_database_code               7241831
_refine_ls_r_f_factor            0.02533
_gsas_proc_ls_prof_r_b_factor    0.01699
_gsas_proc_ls_prof_wr_b_factor   0.02764